#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/22/2202295.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2202295
loop_
_publ_author_name
'Lee, Uk'
'Joo, Hea-Chung'
_publ_section_title
;
 Potassium--sodium double salt of decavanadate,
 K₄Na₂[V₁₀O₂₈]·10H₂O
;
_journal_issue                   8
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i122
_journal_page_last               i124
_journal_paper_doi               10.1107/S1600536803016453
_journal_volume                  59
_journal_year                    2003
_chemical_formula_iupac          'Na2 K4 (V10 O28), 10H2 O'
_chemical_formula_moiety         'O28 V10 6-, 10(H2 O), 4(K) 4+, 2(Na) 2+'
_chemical_formula_structural     'Na2 K4 (V10 O28) (H2 O)10'
_chemical_formula_sum            'H20 K4 Na2 O38 V10'
_chemical_formula_weight         1339.94
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                69.220(10)
_cell_angle_beta                 87.140(10)
_cell_angle_gamma                66.120(10)
_cell_formula_units_Z            1
_cell_length_a                   8.6200(10)
_cell_length_b                   10.3870(10)
_cell_length_c                   11.017(2)
_cell_measurement_reflns_used    28
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      10.5
_cell_measurement_theta_min      9.5
_cell_volume                     838.2(2)
_computing_cell_refinement       STADI4
_computing_data_collection       'STADI4 (Stoe & Cie, 1996)'
_computing_data_reduction        'X-RED (Stoe & Cie, 1996)'
_computing_molecular_graphics
'ORTEP-3 (Farrugia, 1997) and DIAMOND (Brandenburg, 1998)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Stoe Stadi-4'
_diffrn_measurement_method       ω/2-θ
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0171
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            3845
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         1.99
_diffrn_standards_decay_%        3.6
_diffrn_standards_interval_time  60
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    3.302
_exptl_absorpt_correction_T_max  0.534
_exptl_absorpt_correction_T_min  0.317
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   '(X-SHAPE; Stoe & Cie, 1996)'
_exptl_crystal_colour            'pale brown'
_exptl_crystal_density_diffrn    2.654
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'hexagonal prism'
_exptl_crystal_F_000             652
_exptl_crystal_size_max          0.44
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.19
_refine_diff_density_max         0.953
_refine_diff_density_min         -1.077
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.109
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     244
_refine_ls_number_reflns         3845
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.109
_refine_ls_R_factor_all          0.0407
_refine_ls_R_factor_gt           0.0336
_refine_ls_shift/su_max          <0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0418P)²+1.8027P] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0874
_refine_ls_wR_factor_ref         0.0937
_reflns_number_gt                3393
_reflns_number_total             3845
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            br6109.cif
_cod_data_source_block           I
_cod_database_code               2202295
_cod_database_fobs_code          2202295
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_type_symbol
V1 0.31082(6) 0.49974(5) 0.52005(5) 0.01449(12) Uani d . 1 . . V
V2 0.47458(7) 0.20815(6) 0.76614(5) 0.01953(13) Uani d . 1 . . V
V3 0.52954(6) 0.49445(6) 0.74540(5) 0.01700(12) Uani d . 1 . . V
V4 0.82986(6) 0.21084(6) 0.72371(5) 0.01911(13) Uani d . 1 . . V
V5 0.62322(6) 0.21477(6) 0.49938(5) 0.01716(12) Uani d . 1 . . V
K1 -0.18488(10) 0.78857(9) 0.50573(9) 0.03254(18) Uani d . 1 . . K
K2 0.26515(16) 0.81715(13) 0.92705(10) 0.0635(4) Uani d . 1 . . K
Na -0.07082(17) 0.66774(15) 0.86876(13) 0.0279(3) Uani d . 1 . . Na
Oh1 0.4307(2) 0.6251(2) 0.39380(19) 0.0155(4) Uani d . 1 . . O
Oc2 0.3180(3) 0.6169(2) 0.6196(2) 0.0162(4) Uani d . 1 . . O
Oc3 0.3969(3) 0.3805(2) 0.4129(2) 0.0162(4) Uani d . 1 . . O
Ob4 0.1250(3) 0.6252(2) 0.4279(2) 0.0189(4) Uani d . 1 . . O
Ob5 0.2656(3) 0.3680(2) 0.6425(2) 0.0185(4) Uani d . 1 . . O
Ob6 0.7057(3) 0.1162(2) 0.8254(2) 0.0215(4) Uani d . 1 . . O
Ob7 0.4436(3) 0.3577(2) 0.8349(2) 0.0206(4) Uani d . 1 . . O
Ob8 0.7518(3) 0.3614(2) 0.7985(2) 0.0198(4) Uani d . 1 . . O
Ob9 0.5187(3) 0.1299(2) 0.6315(2) 0.0202(4) Uani d . 1 . . O
Ob10 0.8300(3) 0.1321(2) 0.5958(2) 0.0196(4) Uani d . 1 . . O
Ot11 0.3945(3) 0.1030(3) 0.8652(2) 0.0304(5) Uani d . 1 . . O
Ot12 0.4948(3) 0.5977(3) 0.8333(2) 0.0238(5) Uani d . 1 . . O
Ot13 1.0241(3) 0.1100(3) 0.7909(2) 0.0278(5) Uani d . 1 . . O
Ot14 0.6594(3) 0.1132(3) 0.4099(2) 0.0243(5) Uani d . 1 . . O
Ow1 -0.0300(3) 0.5184(3) 0.7436(3) 0.0383(7) Uani d . 1 . . O
Hw1A -0.0939 0.4561 0.7682 0.057 Uiso d R 1 . . H
Hw1B 0.0894 0.4575 0.7409 0.057 Uiso d R 1 . . H
Ow2 0.0289(4) 0.8147(3) 0.7004(3) 0.0533(9) Uani d . 1 . . O
Hw2A 0.1430 0.7690 0.6753 0.080 Uiso d R 1 . . H
Hw2B -0.0140 0.9185 0.6561 0.080 Uiso d R 1 . . H
Ow3 -0.3404(4) 0.8173(3) 0.7436(3) 0.0453(8) Uani d . 1 . . O
Hw3A -0.3906 0.9205 0.7412 0.068 Uiso d R 1 . . H
Hw3B -0.4211 0.7712 0.7680 0.068 Uiso d R 1 . . H
Ow4 0.2044(3) 0.4874(3) 0.9860(2) 0.0315(6) Uani d . 1 . . O
Hw4A 0.2574 0.5278 1.0300 0.047 Uiso d R 1 . . H
Hw4B 0.2828 0.4382 0.9335 0.047 Uiso d R 1 . . H
Ow5 -0.0692(4) 0.8226(3) 0.9772(3) 0.0441(7) Uani d . 1 . . O
Hw5A -0.0779 0.7799 1.0701 0.066 Uiso d R 1 . . H
Hw5B -0.1590 0.9241 0.9392 0.066 Uiso d R 1 . . H
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
V4 V1 V2 2_666 . 176.49(2)
V4 V1 V3 2_666 2_666 60.06(2)
V2 V1 V3 . 2_666 118.27(2)
V4 V1 V5 2_666 2_666 59.56(2)
V2 V1 V5 . 2_666 118.00(2)
V3 V1 V5 2_666 2_666 89.58(2)
V4 V1 V1 2_666 2_666 88.13(2)
V2 V1 V1 . 2_666 88.39(2)
V3 V1 V1 2_666 2_666 58.89(2)
V5 V1 V1 2_666 2_666 58.85(2)
V4 V2 V1 . . 90.85(2)
V5 V3 V4 2_666 . 119.32(2)
V1 V4 V2 2_666 . 92.62(2)
V1 V4 V5 2_666 . 62.03(2)
V2 V4 V5 . . 60.96(2)
V1 V4 V3 2_666 . 61.57(2)
V2 V4 V3 . . 60.547(19)
V5 V4 V3 . . 91.83(2)
V3 V5 V4 2_666 . 119.17(2)
Ob4 V1 Ob5 . . 106.60(10)
Ob4 V1 Oc3 . . 98.10(10)
Ob5 V1 Oc3 . . 96.10(10)
Ob4 V1 Oc2 . . 97.20(10)
Ob5 V1 Oc2 . . 97.00(10)
Oc3 V1 Oc2 . . 156.10(9)
Ob4 V1 Oh1 . . 88.34(9)
Ob5 V1 Oh1 . . 165.08(9)
Oc3 V1 Oh1 . . 81.06(9)
Oc2 V1 Oh1 . . 81.09(9)
Ob4 V1 Oh1 . 2_666 166.70(10)
Ob5 V1 Oh1 . 2_666 86.74(9)
Oc3 V1 Oh1 . 2_666 80.69(8)
Oc2 V1 Oh1 . 2_666 80.24(8)
Oh1 V1 Oh1 . 2_666 78.36(9)
Ot11 V2 Ob6 . . 105.00(10)
Ot11 V2 Ob7 . . 104.10(10)
Ob6 V2 Ob7 . . 89.90(10)
Ot11 V2 Ob9 . . 101.60(10)
Ob6 V2 Ob9 . . 90.90(10)
Ob7 V2 Ob9 . . 153.10(10)
Ot11 V2 Ob5 . . 100.80(10)
Ob6 V2 Ob5 . . 154.10(10)
Ob7 V2 Ob5 . . 84.54(9)
Ob9 V2 Ob5 . . 83.05(9)
Ot11 V2 Oh1 . 2_666 174.70(10)
Ob6 V2 Oh1 . 2_666 80.15(9)
Ob7 V2 Oh1 . 2_666 76.88(8)
Ob9 V2 Oh1 . 2_666 76.83(8)
Ob5 V2 Oh1 . 2_666 73.99(8)
Ot12 V3 Ob8 . . 102.90(10)
Ot12 V3 Ob7 . . 102.90(10)
Ob8 V3 Ob7 . . 94.70(10)
Ot12 V3 Oc2 . . 99.50(10)
Ob8 V3 Oc2 . . 155.07(9)
Ob7 V3 Oc2 . . 90.80(10)
Ot12 V3 Oc3 . 2_666 99.30(10)
Ob8 V3 Oc3 . 2_666 89.57(9)
Ob7 V3 Oc3 . 2_666 155.84(9)
Oc2 V3 Oc3 . 2_666 76.11(9)
Ot12 V3 Oh1 . 2_666 174.00(10)
Ob8 V3 Oh1 . 2_666 80.37(9)
Ob7 V3 Oh1 . 2_666 81.73(9)
Oc2 V3 Oh1 . 2_666 76.37(8)
Oc3 V3 Oh1 2_666 2_666 75.55(8)
Ot13 V4 Ob6 . . 105.10(10)
Ot13 V4 Ob10 . . 100.50(10)
Ob6 V4 Ob10 . . 93.10(10)
Ot13 V4 Ob8 . . 102.50(10)
Ob6 V4 Ob8 . . 90.80(10)
Ob10 V4 Ob8 . . 154.78(9)
Ot13 V4 Ob4 . 2_666 97.50(10)
Ob6 V4 Ob4 . 2_666 157.37(9)
Ob10 V4 Ob4 . 2_666 83.46(9)
Ob8 V4 Ob4 . 2_666 83.43(9)
Ot13 V4 Oh1 . 2_666 171.90(10)
Ob6 V4 Oh1 . 2_666 83.03(9)
Ob10 V4 Oh1 . 2_666 78.46(8)
Ob8 V4 Oh1 . 2_666 77.29(8)
OB4 V4 OH1 2_666 2_666 74.36(8)
Ot14 V5 Ob9 . . 103.40(10)
Ot14 V5 Ob10 . . 102.10(10)
Ob9 V5 Ob10 . . 95.50(10)
Ot14 V5 Oc3 . . 100.70(10)
Ob9 V5 Oc3 . . 89.85(9)
Ob10 V5 Oc3 . . 154.64(9)
Ot14 V5 Oc2 . 2_666 99.80(10)
Ob9 V5 Oc2 . 2_666 154.81(9)
Ob10 V5 Oc2 . 2_666 89.01(9)
Oc3 V5 Oc2 . 2_666 76.27(9)
Ot14 V5 Oh1 . 2_666 174.60(10)
Ob9 V5 Oh1 . 2_666 81.17(9)
Ob10 V5 Oh1 . 2_666 80.18(8)
OC3 V5 OH1 . 2_666 76.17(8)
OC2 V5 OH1 2_666 2_666 75.19(8)
Ob4 K1 Ot14 . 1_465 122.30(7)
Ob4 K1 Oc3 . 2_566 112.37(7)
Ot14 K1 Oc3 1_465 2_566 119.96(7)
Ob4 K1 Ow1 . . 78.12(7)
Ot14 K1 Ow1 1_465 . 143.03(7)
Oc3 K1 Ow1 2_566 . 67.67(7)
Ob4 K1 Ow3 . . 140.35(8)
Ot14 K1 Ow3 1_465 . 83.43(8)
Oc3 K1 Ow3 2_566 . 68.32(7)
Ow1 K1 Ow3 . . 65.40(8)
Ob4 K1 Ob5 . 2_566 73.82(6)
Ot14 K1 Ob5 1_465 2_566 118.88(7)
Oc3 K1 Ob5 2_566 2_566 54.76(6)
Ow1 K1 Ob5 . 2_566 95.43(7)
Ow3 K1 Ob5 . 2_566 122.81(7)
Ob4 K1 Ob9 . 2_566 121.50(7)
Ot14 K1 Ob9 1_465 2_566 76.09(7)
Oc3 K1 Ob9 2_566 2_566 54.43(6)
Ow1 K1 Ob9 . 2_566 122.10(7)
Ow3 K1 Ob9 . 2_566 92.01(7)
Ob5 K1 Ob9 2_566 2_566 51.85(6)
Ob4 K1 Ow2 . . 86.76(7)
Ot14 K1 Ow2 1_465 . 84.94(8)
Oc3 K1 Ow2 2_566 . 122.58(7)
Ow1 K1 Ow2 . . 64.35(8)
Ow3 K1 Ow2 . . 64.30(8)
Ob5 K1 Ow2 2_566 . 154.80(7)
Ob9 K1 Ow2 2_566 . 151.36(7)
Ot13 K2 Ot12 1_465 . 130.18(8)
Ot13 K2 Ow5 1_465 . 72.21(8)
Ot12 K2 Ow5 . . 119.03(9)
Ot13 K2 Ob8 1_465 2_667 123.32(8)
Ot12 K2 Ob8 . 2_667 103.76(7)
Ow5 K2 Ob8 . 2_667 66.59(8)
Ot13 K2 Ob6 1_465 2_667 93.38(7)
Ot12 K2 Ob6 . 2_667 131.44(7)
Ow5 K2 Ob6 . 2_667 91.13(8)
Ob8 K2 Ob6 2_667 2_667 51.80(6)
Ot13 K2 Ob7 1_465 2_667 139.41(8)
Ot12 K2 Ob7 . 2_667 81.64(7)
Ow5 K2 Ob7 . 2_667 118.16(8)
Ob8 K2 Ob7 2_667 2_667 51.65(6)
Ob6 K2 Ob7 2_667 2_667 49.91(6)
Ot13 K2 Ow2 1_465 . 70.10(8)
Ot12 K2 Ow2 . . 75.47(7)
Ow5 K2 Ow2 . . 60.46(8)
Ob8 K2 Ow2 2_667 . 116.26(8)
Ob6 K2 Ow2 2_667 . 150.02(7)
Ob7 K2 Ow2 2_667 . 150.39(7)
Ot13 K2 Ot11 1_465 1_565 63.31(7)
Ot12 K2 Ot11 . 1_565 109.14(8)
Ow5 K2 Ot11 . 1_565 128.60(8)
Ob8 K2 Ot11 2_667 1_565 119.11(7)
Ob6 K2 Ot11 2_667 1_565 68.07(7)
Ob7 K2 Ot11 2_667 1_565 84.28(7)
Ow2 K2 Ot11 . 1_565 120.78(7)
Ow5 Na Ow2 . . 85.10(10)
Ow5 Na Ow1 . . 169.70(10)
Ow2 Na Ow1 . . 86.30(10)
Ow5 Na Ow3 . . 100.00(10)
Ow2 Na Ow3 . . 85.60(10)
Ow1 Na Ow3 . . 84.90(10)
Ow5 Na Ow4 . . 88.10(10)
Ow2 Na Ow4 . . 96.50(10)
Ow1 Na Ow4 . . 87.30(10)
Ow3 Na Ow4 . . 171.80(10)
Ow5 Na Ow4 . 2_567 103.20(10)
Ow2 Na Ow4 . 2_567 169.60(10)
Ow1 Na Ow4 . 2_567 86.00(10)
Ow3 Na Ow4 . 2_567 86.80(10)
Ow4 Na Ow4 . 2_567 90.10(10)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
V1 V1 2_666 3.2710(10) ?
V1 V2 . 3.1001(9) ?
V1 V3 2_666 3.1607(9) ?
V1 V4 2_666 3.0601(9) ?
V1 V5 2_666 3.1725(7) ?
V2 V4 . 3.0847(8) ?
V3 V5 2_666 3.0795(9) ?
V3 V4 . 3.1145(8) ?
V4 V5 . 3.0969(9) ?
V1 Oh1 . 2.088(2) y
V1 Oh1 2_666 2.132(2) y
V1 Oc2 . 1.924(2) y
V1 Oc3 . 1.920(2) y
V1 Ob4 . 1.682(2) y
V1 Ob5 . 1.707(2) y
V2 Oh1 2_666 2.368(2) y
V2 Ob5 . 2.019(2) y
V2 Ob6 . 1.858(2) y
V2 Ob7 . 1.881(2) y
V2 Ob9 . 1.885(2) y
V2 Ot11 . 1.597(2) y
V3 Oh1 2_666 2.228(2) y
V3 Oc2 . 1.997(2) y
V3 Oc3 2_666 2.020(2) y
V3 Ob7 . 1.824(2) y
V3 Ob8 . 1.821(2) y
V3 Ot12 . 1.621(2) y
V4 Oh1 2_666 2.291(2) y
V4 Ob4 2_666 2.072(2) y
V4 Ob6 . 1.822(2) y
V4 Ob8 . 1.893(2) y
V4 Ob10 . 1.864(2) y
V4 Ot13 . 1.613(2) y
V5 Oh1 2_666 2.253(2) y
V5 Oc2 2_666 2.015(2) y
V5 Oc3 . 1.995(2) y
V5 Ob9 . 1.819(2) y
V5 Ob10 . 1.829(2) y
V5 Ot14 . 1.619(2) y
K1 Oc3 2_566 2.923(2) y
K1 Ob4 . 2.807(2) y
K1 Ob5 2_566 2.951(2) y
K1 Ob9 2_566 2.973(2) y
K1 Ot14 1_465 2.870(2) y
K1 Ow1 . 2.937(3) y
K1 Ow2 . 3.047(4) y
K1 Ow3 . 2.938(4) y
K2 Ob6 2_667 3.086(3) y
K2 Ob7 2_667 3.172(2) y
K2 Ob8 2_667 2.966(3) y
K2 Ot11 1_565 3.420(3) y
K2 Ot12 . 2.827(2) y
K2 Ot13 1_465 2.788(3) y
K2 Ow2 . 3.313(4) y
K2 Ow5 . 2.889(4) y
Na Ow1 . 2.337(3) y
Na Ow2 . 2.325(3) y
Na Ow3 . 2.365(3) y
Na Ow4 . 2.407(3) y
Na Ow4 2_567 2.444(3) y
Na Ow5 . 2.324(3) y
Ow1 Hw1a . 0.9714 ?
Ow1 Hw1b . 0.9709 ?
Ow2 Hw2a . 0.9784 ?
Ow2 Hw2b . 0.9265 ?
Ow3 Hw3a . 0.9709 ?
Ow3 Hw3b . 0.9714 ?
Ow4 Hw4a . 0.9704 ?
Ow4 Hw4b . 0.9711 ?
OW5 Hw5a . 0.9730 ?
Ow5 Hw5b . 0.9716 ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
Ow1 Hw1a Ob4 2_566 0.97 2.64 3.100(3) 109
Ow1 Hw1b Ob5 . 0.97 1.94 2.811(3) 148
Ow2 Hw2a Oc2 . 0.98 1.95 2.856(3) 152
Ow2 Hw2b Ob10 1_465 0.93 1.95 2.839(4) 160
Ow3 Hw3a Ob9 1_465 0.97 1.91 2.767(3) 146
Ow3 Hw3b Ot14 2_566 0.97 2.50 2.989(4) 111
Ow4 Hw4b Ob7 . 0.97 1.83 2.799(3) 174
Ow4 Hw4a Ot12 2_667 0.97 2.28 2.980(3) 128
Ow5 Hw5b Ob6 1_465 0.97 1.84 2.789(4) 163
Ow5 Hw5a Ot13 2_667 0.97 2.37 2.959(4) 119
